Enhanced Organic Pollutant Removal Efficiency of Electrospun NiTiO3/TiO2-Decorated Carbon Nanofibers

A nanocomposite comprised of nickel titanate/titania nanoparticles decorated with carbon nanofibers (NiTiO3/TiO2-decorated CNFs) is successfully synthesized via electrospinning and further utilized for methylene blue (MB) photodegradation. The morphology, phase, structural and chemical composition of the nanocomposite is investigated via scanning electron microscope, X-ray diffraction and transmission electron microscope equipped with energy dispersive X-ray. A mathematical model is developed to predict the photocatalytic activity of the produced nanocomposite by considering parameters such as initial dye concentration, light intensity, reaction temperature, and catalyst dosage. The reaction rate constant K1 decreased from 0.0153 to 0.0044 min−1 with an increase in the MB concentration from 5 to 15 mg L−1, while K2, K3, and K4 were found to increase with the increase in reaction temperature (0.0153 to 0.0222 min−1), light intensity (0.0153 to 0.0228 min−1) and catalyst dose concentration (0.0153 to 0.0324 min−1), respectively. The results obtained are found to be in good agreement with the modeling results and showed effective photodegradation activity. The performance of our catalyst is found to be better compared to other catalysts previously reported in the literature. The recyclability data of the synthesized NiTiO3/TiO2-decorated CNFs catalyst for four runs show that the catalyst is quite stable and recyclable. This nanocomposite photocatalyst offers a low-cost solution for wastewater pollution problems and opens new avenues to further explore the electrospinning method for the synthesis of nanocomposites.


Introduction
Organic pollutants produced from industrial water pose a serious threat to our environment, which will eventually affect the health of humans and aquatic life [1][2][3]. Therefore, solving this problem calls for urgent attention to not only get rid of these pollutants but also to overcome the shortage of usable fresh water. According to the UNESCO World Water Assessment Program (2003), about 2 million tons of disposed water from industrial and agricultural sources is released every day [4]. Thus, recycling and reusing disposed water has become a necessity. However, an effective and safe method to obtain usable water requires a high cost. Traditional methods such as chemical coagulation, flocculation, and adsorption have been employed to overcome the aforementioned issue; however, these methods suffer a major drawback in the formation of a secondary pollutant, and thus require additional steps to remove this, incurring an additional cost [5][6][7][8][9]. The photocatalytic process utilizing semiconducting materials is considered as an eco-friendly and inexpensive method for the decomposition and mineralization of untreated pollutants resulting from industrial wastewater employing ultraviolet or visible light irradiation [10,11]. Several photocatalytic semiconductors are being used in the decomposition of organic and inorganic pollutants. Titanium dioxide (TiO 2 ) is the most common semiconductor utilized in the photocatalytic processes such as dye-sensitized solar cells (DSSC), photodegradation of untreated pollutants, self-cleaning paint, and water splitting [12][13][14]. TiO 2 is a low-cost material which is chemically stable, environmentally compatible, and easily available.
in advance by dissolving 1.0 g of PVP in 10 mL deionized water at room temperature for 2 h duration under agitation. The poly(vinylpyrrolidone) solution was prepared as mentioned in previous reports [34][35][36][37][38][39]. The mixture was stirred until a transparent yellow gel was obtained. Then, nickel acetate tetrahydrate was added to this gel and continuously stirred until a green transparent gel was obtained. The prepared gel was fed into the plastic syringe of the lab-scale electrospinning device (NaBond Technologies Co., Limited, Hi Tech Park, Nanshan Dist., Shenzhen, Guangdong, China). The positive electrode was connected to the metallic end of the plastic syringe while the negative electrode was attached to the aluminum foil wrapped around the rotating cylinder. The voltage and distance between the positive and negative electrode during the spinning process were maintained at 20 kV and 15 cm, respectively. The NF mats formed on the surface of the aluminum foil were detached and placed in a vacuum dryer at a temperature of 50 • C for 24 h to get rid of the solvents. This was then calcined at 800 • C for 5 h. This synthesized material was named NiTiO 3 /TiO 2 -decorated CNFs. The TiO 2 @CNFs were prepared using a similar procedure except that the nickel acetate tetrahydrate was not added during gel preparation.

Catalyst Characterization
The morphological study of the NiTiO 3 /TiO 2 -decorated CNFs was performed by employing a scanning electron microscope (SEM Model JSM-5900, Japan Electron Optics Laboratory (JEOL Ltd., Tokyo, Japan) equipped with energy dispersive X-ray spectroscopic analysis (EDX). The crystallinity of the NFs was studied using an X-ray diffractometer (XRD, Rigaku Co., Tokyo, Japan) with Cu Kα radiation (λ = 1.54056 Å) in the range of 10 • to 80 • of two theta angles. A high-resolution transmission electron microscope (HRTEM) image was captured via JEOL Model JEM-2200FS, operated at 200 kV and equipped with EDX (JEOL Ltd., Tokyo, Japan).

Determination of MB Photodegradation
The MB photo-degradation in the presence of NiTiO 3 /TiO 2 -decorated CNFs was carried out in a simple batch photo-reactor consisting of a simple laboratory borosilicate glass bottle (150 mL). A visible fluorescent lamp was used as the light source (λ= 420-700 nm, I = 23-40 Wm −2 (Philips Co., Amsterdam, The Netherlands). The reactor (150 mL borosilicate glass bottle) was charged with 100 mL of MB aqueous solution with known concentration and a previously known amount of NiTiO 3 /TiO 2 -decorated CNFs photocatalyst. The solution was kept in the dark under continuous stirring for 20 min to determine the adsorption-desorption capacity of the photocatalyst towards MB. Later, the solution was stirred and exposed directly to the visible light radiation. The distance between the reactor and the lamp was 12 cm. The reaction temperature was controlled via a thermostat water bath. An aliquot of 3.0 mL of MB solution was withdrawn after specific time intervals under irradiation. The solution sample was centrifuged to separate the solid catalyst from the solution. Then, the filtered solution was introduced into a UV-visible spectrophotometer to determine the MB concentration present in the solution. The reaction parameters studied were MB concentration, reaction temperature, light intensity and the catalyst concentration. Figure 1A displays the SEM image of the electrospun nanofiber mat consisting of nickel acetate tetrahydrate, titanium isopropoxide, and poly(vinylpyrrolidone) after vacuum drying at 50 • C for 24 h. The image shows smooth and bead-free NFs. During the calcination process performed at 800 • C, NFs preserved their structure with the growth of tiny white NPs on the surface of NFs ( Figure 1B). EDX analysis (Inset Figure 1B) indicates that the NFs mainly consisted of nickel (Ni), titanium (Ti), oxygen (O), and carbon (C), with the absence of any other element. tiny white NPs on the surface of NFs ( Figure 1B). EDX analysis (Inset Figure 1B) indicates that the NFs mainly consisted of nickel (Ni), titanium (Ti), oxygen (O), and carbon (C), with the absence of any other element.   107), and (211) crystal planes, respectively. The low intensity peak observed at 2θ value of 32.4° is in agreement with the (002) plane of carbon-like graphite, which is formed due to the partial decomposition of carbon during the calcination process. TEM EDX was performed to determine the chemical composition of synthesized NFs ( Figure 3). Figure 3A displays the TEM image of a single selected NF along with the line TEM-EDX analysis and the corresponding EDX analysis is displayed in Figure 3B-E. It is evident from the figure that Ti, O, Ni, and C have the same distribution, which confirmed the formation of the NiTiO3-TiO2 composite. The carbon was covered with NiTiO3-TiO2  Polymers 2023, 14, x FOR PEER REVIEW 4 tiny white NPs on the surface of NFs ( Figure 1B). EDX analysis (Inset Figure 1B) ind that the NFs mainly consisted of nickel (Ni), titanium (Ti), oxygen (O), and carbo with the absence of any other element.  TEM EDX was performed to determine the chemical composition of synthesize ( Figure 3). Figure 3A displays the TEM image of a single selected NF along with th TEM-EDX analysis and the corresponding EDX analysis is displayed in Figure 3B-E evident from the figure that Ti, O, Ni, and C have the same distribution, which confi the formation of the NiTiO3-TiO2 composite. The carbon was covered with NiTiO TEM EDX was performed to determine the chemical composition of synthesized NFs ( Figure 3). Figure 3A displays the TEM image of a single selected NF along with the line TEM-EDX analysis and the corresponding EDX analysis is displayed in Figure 3B-E. It is evident from the figure that Ti, O, Ni, and C have the same distribution, which confirmed the formation of the NiTiO 3 -TiO 2 composite. The carbon was covered with NiTiO 3 -TiO 2 composite ( Figure 3A). The presence of carbon may be enhancing the overall photocatalytic process through the enhanced photo-induced e − and h + separation, the more exposed area to the pollutant and the enhanced photodegradation rate. composite ( Figure 3A). The presence of carbon may be enhancing the overall photocatalytic process through the enhanced photo-induced e − and h + separation, the more exposed area to the pollutant and the enhanced photodegradation rate.

Photocatalytic Degradation of MB
To understand the photodegradation process of MB dye using NiTiO3/TiO2-decorated CNFs catalyst, we considered the effect of MB dye concentration (Ci), reaction temperature (T), photocatalyst dosage (NiTiO3/TiO2-decorated CNFs), and light intensity (I). The following mathematical model is designed to predict the photocatalytic reaction as a function of the studied parameters [40]:

Photocatalytic Degradation of MB
To understand the photodegradation process of MB dye using NiTiO 3 /TiO 2 -decorated CNFs catalyst, we considered the effect of MB dye concentration (C i ), reaction temperature (T), photocatalyst dosage (NiTiO 3 /TiO 2 -decorated CNFs), and light intensity (I). The following mathematical model is designed to predict the photocatalytic reaction as a function of the studied parameters [40]: (1) Figure 4 shows the change of MB concentration versus irradiation time in the absence of photocatalytic NFs, and in the presence of TiO 2 @CNFs and NiTiO 3 /TiO 2 @CNFs. It can be observed from Figure 4 that the efficiency of MB photodegradation using NiTiO 3 /TiO 2decorated CNFs is higher than that of TiO 2 @CNFs. After 120 min of visible light irradiation, enhanced photodegradation of 82.4% and 62.5% is achieved for NiTiO 3 /TiO 2 -decorated CNFs and TiO 2 @CNFs, respectively. This achievement of 20% increase in photodegradation activity is significant. TiO 2 alone is not very active under visible irradiation, however when TiO 2 is doped with carbon, the band gap of titania narrows which makes it active under visible irradiation [3].
Polymers 2023, 14, x FOR PEER REVIEW 6 of 18 Figure 4 shows the change of MB concentration versus irradiation time in the absence of photocatalytic NFs, and in the presence of TiO2@CNFs and NiTiO3/TiO2@CNFs. It can be observed from Figure 4 that the efficiency of MB photodegradation using NiTiO3/TiO2decorated CNFs is higher than that of TiO2@CNFs. After 120 min of visible light irradiation, enhanced photodegradation of 82.4% and 62.5% is achieved for NiTiO3/TiO2-decorated CNFs and TiO2@CNFs, respectively. This achievement of 20% increase in photodegradation activity is significant. TiO2 alone is not very active under visible irradiation, however when TiO2 is doped with carbon, the band gap of titania narrows which makes it active under visible irradiation [3].

Effect of Initial Dye Concentration (Ci)
We studied the effect of initial MB dye concentration (5, 7.5, 10, and 15 mg L −1 ) on the photodegradation reaction under visible light irradiation in the presence of NiTiO3/TiO2decorated CNFs. As seen in Figure 5A, the MB photodegradation decreases with increasing MB concentration, which may be plausibly due to the limited production of active radicals in the photocatalytic process at higher MB concentrations [30,41]. Furthermore, higher concentration of MB dye could absorb more light and cause the prevention of photons to reach to the surface of the photocatalyst, thereby reducing the efficiency of the photodegradation process [42][43][44]. Thus, the photodegradation process is efficient at low concentrations because of more available active sites on the surface of the photocatalyst to adsorb dye molecules. Photodegradation of organic compounds can be described through a pseudo-first order reaction according to the Langmuir Hinshelwood (LH) model (Equation (2)).

Effect of Initial Dye Concentration (C i )
We studied the effect of initial MB dye concentration (5, 7.5, 10, and 15 mg L −1 ) on the photodegradation reaction under visible light irradiation in the presence of NiTiO 3 /TiO 2decorated CNFs. As seen in Figure 5A, the MB photodegradation decreases with increasing MB concentration, which may be plausibly due to the limited production of active radicals in the photocatalytic process at higher MB concentrations [30,41]. Furthermore, higher concentration of MB dye could absorb more light and cause the prevention of photons to reach to the surface of the photocatalyst, thereby reducing the efficiency of the photodegradation process [42][43][44]. Thus, the photodegradation process is efficient at low concentrations because of more available active sites on the surface of the photocatalyst to adsorb dye molecules. Photodegradation of organic compounds can be described through a pseudo-first order reaction according to the Langmuir Hinshelwood (LH) model (Equation (2)).    Figure 5A shows the kinetics of the MB degradation over the NiTiO 3 /TiO 2 -decorated CNFs at various concentrations. The value of rate constant (K 1 ) can be determined from the slope of the straight line obtained in Figure 5B. The value of K 1 decreases from 0.0153 to 0.0044 min −1 with the increase of MB concentration from 5 to 15 mg L −1 (Table 1), which may be plausibly due to the limited formation of active radicals at higher concentrations. The relationship between K 1 and C i is obtained via a 1/K 1 versus C i plot ( Figure 5B) and modified LH model by transforming Equation (6).
to a straight-line equation  Figure 6A depicts the variation of photodegradation of MB versus irradiation time at various reaction temperatures. As shown in the figure, the photodegradation of MB increased with the increase in reaction temperature from 25 to 40 • C due to improved charge transfer at higher temperatures. The movement of electron-hole pairs becomes more active as the reaction temperature increases, which leads to the reaction between electrons, adsorbed oxygen and holes, and faster generation of hydroxyl radicals and hydroxyl ions, consequently improving the photodegradation of MB dye [45][46][47]. The temperature range of 20-80 • C is considered best for the effective photodegradation of organic compounds [45,48]. Further increases in the temperature could reduce the photocatalytic activity since the electron-hole recombination rate increased [45]. At the same time, low reaction temperature leads to reduction in the solubility of MB in water, causing partial condensation of MB in water [45,49].

Effect of Light Intensity (I)
The photodegradation rate of organic compounds is affected by the light intensity and wavelength [42,[50][51][52]. Figure 7A shows the influence of light intensity on the MB photodegradation. It is evident from the figure that the rate of MB photodegradation increased with the increase in light intensity. An increase in light intensity means the availability of a large number of photons, which improved the MB photodegradation. The rate constant (K3) can be determined from the slope of straight lines obtained from the plot of ln (Ci/Cf) versus time at various light intensities ( Figure 7A). The value of K3 increased from 0.0153 to 0.0228 min −1 with the increase in light intensities from 25 to 40 Wm −2 (Table  1), which indicates an enhancement in the MB photodegradation with increasing light intensity. The correlation between K3 and I is obtained by plotting 1/K1 versus I ( Figure  7B) and applying Equation (9) [40], since K3 is directly proportional to I as demonstrated in the following relationship: K = mI   Figure 6B shows the kinetic study of MB photodegradation over the NiTiO 3 /TiO 2decorated CNFs at various temperatures. The value of reaction rate (K 2 ) increased from 0.0153 to 0.0222 min −1 with the increase of reaction temperature from 25 to 40 • C (Table 1), indicating an enhancement in the MB photodegradation efficiency with increasing temperature due to higher charge mobility. The rate constant (K 2 ) can be determined from the slope of the straight line obtained in Figure 6B. The plot of K 2 versus 1/T gives a straight-line relationship. We apply the Arrhenius equation Equation (7) to obtain the activation energy (E a ) of the photocatalytic reaction.
Applying the natural log (Ln) to both sides of Equation (7) removes the exponent to obtain Equation (8) as follows: Transforming Equation (8)

Effect of Light Intensity (I)
The photodegradation rate of organic compounds is affected by the light intensity and wavelength [42,[50][51][52]. Figure 7A shows the influence of light intensity on the MB photodegradation. It is evident from the figure that the rate of MB photodegradation increased with the increase in light intensity. An increase in light intensity means the availability of a large number of photons, which improved the MB photodegradation. The rate constant (K 3 ) can be determined from the slope of straight lines obtained from the plot of ln (C i /C f ) versus time at various light intensities ( Figure 7A). The value of K 3 increased from 0.0153 to 0.0228 min −1 with the increase in light intensities from 25 to 40 Wm −2 (Table 1), which indicates an enhancement in the MB photodegradation with increasing light intensity. The correlation between K 3 and I is obtained by plotting 1/K 1 versus I ( Figure 7B) and applying Equation (9) [40], since K 3 is directly proportional to I as demonstrated in the following relationship: Transforming Equation (9)

Effect of Light Intensity (I)
The photodegradation rate of organic compounds is affected by the light intensity and wavelength [42,[50][51][52]. Figure 7A shows the influence of light intensity on the MB photodegradation. It is evident from the figure that the rate of MB photodegradation increased with the increase in light intensity. An increase in light intensity means the availability of a large number of photons, which improved the MB photodegradation. The rate constant (K3) can be determined from the slope of straight lines obtained from the plot of ln (Ci/Cf) versus time at various light intensities ( Figure 7A). The value of K3 increased from 0.0153 to 0.0228 min −1 with the increase in light intensities from 25 to 40 Wm −2 (Table  1), which indicates an enhancement in the MB photodegradation with increasing light intensity. The correlation between K3 and I is obtained by plotting 1/K1 versus I ( Figure  7B) and applying Equation (9) [40], since K3 is directly proportional to I as demonstrated in the following relationship: K = mI (9) Transforming Equation (9) Figure 8A shows the variation of MB concentration versus irradiation time at various NiTiO 3 /TiO 2 -decorated CNFs doses (200, 300, 400, and 500 mg L −1 ). As evident from the figure, the MB photodegradation increases with the increase in NiTiO 3 /TiO 2 -decorated CNFs dose, which may be plausibly due to increases in the available surface area of the NiTiO 3 /TiO 2 -decorated CNFs that improved the MB photodegradation. Furthermore, it is observed that the MB photodegradation at 400 mg L −1 is very close to the dose at 500 mg L −1 . This could be plausibly due to decreases in the active sites resulting from the aggregation phenomenon at high doses of NiTiO 3 /TiO 2 -decorated CNFs. This also causes light scattering and screening effects that decrease the photoreactions and active radicals [30,[53][54][55]. Figure 8B shows the kinetic study of MB photodegradation over NiTiO 3 /TiO 2 -decorated CNFs at various catalyst doses. The value of reaction rate (K 4 ) increases from 0.0153 to 0.0324 min −1 with the increase in the photocatalyst dose from 200 to 500 mg L −1 (Table 1), indicating an improvement in the MB photodegradation because an increased NiTiO 3 /TiO 2 -decorated CNFs dose provides comparatively high active catalytic sites on the surface. The influence of NiTiO 3 /TiO 2 -decorated CNFs dosage on K 4 is determined by employing a Langmuir-type relationship, Equation (10) [40,56]:

Effect of Photocatalyst Dose (NiTiO 3 /TiO 2 -Decorated CNFs)
This equation can be transformed to a straight-line equation, Equation (11), as follows: The straight-line equation is gation phenomenon at high doses of NiTiO3/TiO2-decorated CNFs. This also causes light scattering and screening effects that decrease the photoreactions and active radicals [30,[53][54][55]. Figure 8B shows the kinetic study of MB photodegradation over NiTiO3/TiO2decorated CNFs at various catalyst doses. The value of reaction rate (K4) increases from 0.0153 to 0.0324 min −1 with the increase in the photocatalyst dose from 200 to 500 mg L −1 ( This equation can be transformed to a straight-line equation, Equation (11), as follows: The straight-line equation is y = ax + b, where x = 1 C ⁄ b = 1 K ⁄ K = 1 3.042 = 0.3287 ⁄ a = 1 K K ⁄ K = 1 (17055 × 0.3287) = 1.783 × 10 ⁄  Figure 9 shows the low-and high-magnification SEM images after using 500 mgL −1 catalyst dosage. As seen in the figure, the photocatalyst kept the nanofibrous structure intact after the photodegradation process. This shows the stability of the nanofibrous catalyst.  Figure 9 shows the low-and high-magnification SEM images after using 500 mg L −1 catalyst dosage. As seen in the figure, the photocatalyst kept the nanofibrous structure intact after the photodegradation process. This shows the stability of the nanofibrous catalyst.

Development of Model Rate Equation
The aforementioned results indicate that the rate constant is a function of MB concentration, reaction temperature, light intensity, and NiTiO3/TiO2-decorated CNFs dose according to Equations (6), (8), (9) and (11

Development of Model Rate Equation
The aforementioned results indicate that the rate constant is a function of MB concentration, reaction temperature, light intensity, and NiTiO 3 /TiO 2 -decorated CNFs dose according to Equations (6), (8), (9) and (11). The determined values of K R , E a , m, and K cat employing multiple regression analysis are shown in Table 2. The equation constant k is calculated using Equation (2) by substituting the previously obtained values of C i , T, I, C TiO2 and values from  A comparison between the experimental data and the determined K app for the MB photodegradation at various conditions is shown in Figure 10. The obtained plot shows that the experimental data are in good agreement with the model-calculated data, which confirms the authenticity of our model to predict the reaction rate constant at various operational conditions.

Photocatalytic Mechanism
The photocatalytic mechanism is proposed for the NiTiO3/TiO2-decorated CNFs in the photodegradation of MB dye. The band alignment and charge transfer diagram of the NiTiO3/TiO2-decorated CNFs is shown in Figure 11. The photocatalytic process is responsible for the production of active radicals and ions. However, the higher bandgap of TiO2 is responsible for the production of fewer active radicals in visible light [57].
The separation of the photogenerated electron-hole pairs across the NiTiO3/TiO2decorated CNFs may be ascertained by calculating the conduction band (CB) and valence band (VB) potentials of the components. Specifically, these energies are calculated using the following empirical formulae: where the VB potential is denoted by EVB, and the CB potential is denoted by ECB. E e is the energy of free electrons versus NHE, which is 4.5 eV [57,58]. Eg is the band gap energy of the semiconductor. Finally, the electronegativity of the semiconductor is denoted by the

Photocatalytic Mechanism
The photocatalytic mechanism is proposed for the NiTiO 3 /TiO 2 -decorated CNFs in the photodegradation of MB dye. The band alignment and charge transfer diagram of the NiTiO 3 /TiO 2 -decorated CNFs is shown in Figure 11. The photocatalytic process is responsible for the production of active radicals and ions. However, the higher bandgap of TiO 2 is responsible for the production of fewer active radicals in visible light [57].
The separation of the photogenerated electron-hole pairs across the NiTiO 3 /TiO 2decorated CNFs may be ascertained by calculating the conduction band (CB) and valence band (VB) potentials of the components. Specifically, these energies are calculated using the following empirical formulae: where the VB potential is denoted by E VB , and the CB potential is denoted by E CB . E e is the energy of free electrons versus NHE, which is 4.5 eV [57,58]. E g is the band gap energy of the semiconductor. Finally, the electronegativity of the semiconductor is denoted by the letter χ. In the conduction band:

Catalyst Recyclability Data
The stability and recyclability of the synthesized NiTiO3/TiO2-decorated CNFs catalyst is tested for MB photodegradation. Figure 12 shows the catalyst recyclability data of the catalyst after 120 min of visible light irradiation for four consecutive runs. The photodegradation activity of the catalyst showed very little decrease (~1.3%) after four runs. The data show that the catalyst is stable and recyclable. The conduction band (CB) and valence band (VB) potentials of NiTiO 3 with respect to the standard hydrogen electrode (SHE) are 0.23 eV and +2.62 eV, respectively [58]. The NiTiO 3 has smaller bandgap (2.62 eV) than pure TiO 2 (3.2 eV), thus the VB position of NiTiO 3 is higher than TiO 2 (+2.7 eV), which enables the hole transfer from the VB of NiTiO 3 to the VB of TiO 2 . The resulting photogenerated hole (h + ) reacts with H 2 O/OHto produce hydroxyl radicals [30,59], while CB of NiTiO 3 is located at a lower position than that of TiO 2 . As light irradiates, the electrons in the VB of NiTiO 3 get excited and reach CB, which results in partial vacancy in the VB, and the electrons from the CB of TiO 2 get transferred to the CB of NiTiO 3 . The role of NiTiO 3 in the photocatalytic mechanism suggests that it can be used as an efficient sensitizer under visible light. The photogenerated electrons in NiTiO 3 move freely towards the surface of the CNFs, suggesting the low recombination of photogenerated electrons and holes [60]. The oxygen molecules react with the photogenerated electrons in the CB of NiTiO 3 to produce • O 2− without recombining with the holes present on the surface of TiO 2 [36]. The resulting • O 2− react with the hydrogen ion and produce HOO • , which consequently alter the MB molecule in the solution. The achieved photocatalytic activity of the NiTiO 3 /TiO 2 heterojunction is higher than that of the pure TiO 2 [61]. The photodegradation mechanism of MB using NiTiO 3 /TiO 2 -decorated CNFs can be explained as follows [1,30]: In the conduction band:

Catalyst Recyclability Data
The stability and recyclability of the synthesized NiTiO3/TiO 2 -decorated CNFs catalyst is tested for MB photodegradation. Figure 12 shows the catalyst recyclability data of the catalyst after 120 min of visible light irradiation for four consecutive runs. The photodegradation activity of the catalyst showed very little decrease (~1.3%) after four runs. The data show that the catalyst is stable and recyclable.

Comparison of Our Results with the Literature
The results obtained from the photocatalytic degradation of MB in the presence of catalyst NiTiO3/TiO2-decorated CNFs is compared with the catalysts reported in the literature with titanate as an active ingredient. The results are reported in Table 3. Marco Alejandro Ruiz Preciado demonstrated the photocatalytic activity of NiTiO3 for the photodegradation of MB using thin films under visible light [62]. Their study determined a reaction rate constant of 0.0030 min −1 . Dao et al. synthesized co-doped NiTiO3/g-C3N4 composite photocatalysts and used them for MB photodegradation under visible light irradiation [63]. The combination of co-doped NiTiO3 and g-C3N4 enhanced the photocatalytic performance of the composite photocatalyst. The co-doped composite photocatalyst (1% co-doped NiTiO3/g-C3N4) produced a higher kapp value (0.0072 min −1 ), while the one loaded with 3% co-doped NiTiO3/g-C3N4 showed a lower value of the rate constant (0.0057 min −1 ). Kitchamsetti [65]. The results showed that the NiTiO3 NPs/MCM-41 composite has higher photocatalytic activity than that of NiTiO3 NPs and exhibited a kinetic rate constant of 0.018 min −1 . Khan et al. synthesized one-dimensional NiTiO3 NFs via electrospinning method and loaded them with acetic acid-treated, exfoliated and sintered sheets of graphitic carbon nitride (AAs-gC3N4), which produced a unique heterogeneous structure [66]. The weight ratio of NiTiO3 NFs to porous AAs-gC3N4 was 40:60, and displayed very good photodegradation of MB at a rate constant of 0.0310 min −1 . This comparison clearly showed that the NiTiO3/TiO2-decorated CNFs catalyst possesses a high kinetic rate constant (0.0324 min −1 ) compared to other reported catalysts.

Comparison of Our Results with the Literature
The results obtained from the photocatalytic degradation of MB in the presence of catalyst NiTiO 3 /TiO 2 -decorated CNFs is compared with the catalysts reported in the literature with titanate as an active ingredient. The results are reported in Table 3. Marco Alejandro Ruiz Preciado demonstrated the photocatalytic activity of NiTiO 3 for the photodegradation of MB using thin films under visible light [62]. Their study determined a reaction rate constant of 0.0030 min −1 . Dao et al. synthesized co-doped NiTiO 3 /g-C 3 N 4 composite photocatalysts and used them for MB photodegradation under visible light irradiation [63]. The combination of co-doped NiTiO 3 and g-C 3 N 4 enhanced the photocatalytic performance of the composite photocatalyst. The co-doped composite photocatalyst (1% co-doped NiTiO 3 /g-C 3 N 4 ) produced a higher k app value (0.0072 min −1 ), while the one loaded with 3% co-doped NiTiO 3 /g-C 3 N 4 showed a lower value of the rate constant (0.0057 min −1 ). Kitchamsetti [65]. The results showed that the NiTiO 3 NPs/MCM-41 composite has higher photocatalytic activity than that of NiTiO 3 NPs and exhibited a kinetic rate constant of 0.018 min −1 . Khan et al. synthesized one-dimensional NiTiO 3 NFs via electrospinning method and loaded them with acetic acid-treated, exfoliated and sintered sheets of graphitic carbon nitride (AAs-gC 3 N 4 ), which produced a unique heterogeneous structure [66]. The weight ratio of NiTiO 3 NFs to porous AAs-gC 3 N 4 was 40:60, and displayed very good photodegradation of MB at a rate constant of 0.0310 min −1 . This comparison clearly showed that the NiTiO 3 /TiO 2 -decorated CNFs catalyst possesses a high kinetic rate constant (0.0324 min −1 ) compared to other reported catalysts. Table 3. Performance comparison of our catalyst with those reported in the literature.

Conclusions
Electrospinning and calcination methods are utilized in the successful synthesis of NiTiO 3 /TiO 2 -decorated CNFs. The chemical composition, structural information, and phase analysis are evaluated via characterization techniques which confirm the fabrication of CNFs. Several operational parameters for the photodegradation application, such as the effect of the initial dye concentration, reaction temperature, light intensity, and catalyst dose, are considered. A successful model is achieved through the determination of reaction rate constant (k app ) to predict the photocatalytic activity of the composite NiTiO 3 /TiO 2decorated CNFs towards photodegradation of MB dye under visible light in a batch reactor. The photodegradation is 82.4% and 62.5% for NiTiO 3 /TiO 2 -decorated CNFs and TiO 2 @CNFs, respectively, after 120 min visible light irradiation. The reaction constants K 1 , K 2 , K 3 , and K 4 determined for initial dye concentration, reaction temperature, light intensity, and photocatalyst dose, respectively, are in full agreement with the estimated results from the model for the rate constant (k app ). The results suggest further exploration of the electrospinning fabrication method for the synthesis and use of NiTiO 3 /TiO 2 -decorated CNFs towards effective photocatalytic activity and future applications in environmental remediation. The recyclability data of the synthesized NiTiO 3 /TiO 2 -decorated CNFs catalyst show that the catalyst is quite stable, and a very small decrease is observed in the MB photodegradation activity from 82.4 to 81.1% after 120 min of visible light irradiation for four consecutive runs. The data also showed good recyclability characteristics of the catalyst. The performance of our catalyst for MB photocatalytic degradation is compared with those reported in the literature and the NiTiO 3 /TiO 2 -decorated CNFs exhibit higher rate constant compared to other catalysts.

Data Availability Statement:
The data presented in this study are available from the corresponding author upon reasonable request.